Download presentation

Presentation is loading. Please wait.

Published byViolet Ford Modified about 1 year ago

1
Magnetism (FM, AFM, FSM) Karlheinz Schwarz Institute of Materials Chemistry TU Wien

2
Localized vs. itinerant systems In localized systems (e.g. some rare earth) the magnetism is mainly governed by the atom (Hund‘s rule) In itinerant (delocalized) systems (many transition metals) magnetism comes from partial occupation of states, which differ between spin-up and spin-down. Boarderline cases (some f-electron systems) details of the structure (e.g. lattice spacing) determine whether or not some electrons are localized or itinerant.

3
Ferro-, antiferro-, or ferri-magnetic Ferromagnetic (FM) (e.g. bcc Fe) M > 0 Antiferromagnetic (AFM) (e.g. Cr) M = 0 Ferrimagnetic cases the moments at different atoms are antiparallel but of different magnitude M > 0 Non-collinear magnetism (NCM) the magnetic moments are not ligned up parallel.

4
Itinerant electron magnetism Experimental facts: Curie temperature

5
Stoner theory of itinerant electron magnetism 1.The carriers of magnetism are the unsaturated spins in the d-band. 2.Effects of exchange are treated with a molecular field term. 3. One must conform to Fermi statistics. Stoner, 1936

6
Stoner model for itinerant electrons In a non magnetic (NM) case N ↑ = N ↓ (spin-up and spin-down) ferromagnetic (FM) case N ↑ > N ↓ (majority and minority spin) the moments at all sites are parallel (collinear) the (spin) magnetic moment m m = N ↑ - N ↓ its orientation with respect to the crystal axes is only defined by spin orbit coupling. there can also be an orbital moment it is often suppressed in 3d transition metals Exchange splitting spin-down spin-up exchange interaction Stoner criterion

7
Stoner model for itinerant electrons The existence of ferromagnetism (FM) is governed by the Stoner criterion I. N(E F ) > 1 N(E F ) DOS at E F (of NM case) I Stoner parameter ~ independent of structure Ferromagnetism appears when the gain in exchange energy is larger than the loss in kinetic energy 1 1 I Fe I Ni P.James, O.Eriksson, B.Johansson, I.A.Abrikosov, Phys.Rev.B 58,... (1998) (a) Fe (b) Ni

8
bcc Fe Non magnetic case EFEF ferromagnetic case EFEF spin-up spin-down spin-up spin-down Exchange splitting E F at high DOS

9
DFT ground state of iron LSDA NM fcc in contrast to experiment GGA FM bcc Correct lattice constant Experiment FM bcc GGA LSDA

10
Iron and its alloys Fe: weak ferromagnet (almost) Co: strong ferromagnet

11
Magnetism and crystal structure V. Heine: „metals are systems with unsaturated covalent bonds“

12
Covalent magnetism Fe-Co alloys e.g. Fe-Co alloys Wigner delay times

13
Spin projected DOS of Fe-Co alloys The alloy is represented by ordered structures Fe 3 Co and FeCo 3 (Heusler) FeCo Zintl or CsCl Fe, Co bcc % Co

14
Iron and its alloys Itinerant or localized?

15
Magnetization density difference between Majoity spin Minority spin Localized around Fe and Co slightly negative between the atoms Itinerant electrons Magnetization density in FeCo CsCl structure m(r)=ρ (r)-ρ (r) K.Schwarz, P.Mohn, P.Blaha, J.Kübler, Electronic and magnetic structure of bcc Fe-Co alloys from band theory, J.Phys.F:Met.Phys. 14, 2659 (1984)

16
Bonding by Wigner delay time single scatterer (Friedel) V(r)=0 solution: NeumannBessel R l joined in value and slope defines phase shift : Friedel sum Wigner delay time

17
Phase shifts, Wigner delay times of Fe, Co, Ni Wigner delay time Phase shifts resonance states

18
Covalent magnetism in FeCo For spin up Fe and Co equivalent partial DOS similar typical bcc DOS For spin down Fe higher than Co Wigner delay time Fe Co bonding antibonding Co No charge transfer between Fe and Co

19
Magnetism and crystal structure Covalent magnetism, FeCo:

20
Antiferromagnetic (AFM) Cr Cr has AFM bcc structure There is a symmetry it is enough to do the spin-up calculation spin-down can be copied Cr 1 Cr 2 Cr 1 Cr 2 spin-up spin-down EFEF Cr 1 = Cr 2 Cr 2 = Cr 1

21
Zeolite, sodalite Al-silicate corner shared SiO 4 tetrahedra AlO 4 tetrahedra cage Al / Si ratio 1 alternating ordered (cubic) 3 e - per cage Si Al

22
SES Sodium electro sodalite Si-Al zeolite (sodalite) Formed by corner-shared SiO 4 and AlO 4 tetrahedra Charge compensated by doping with 4 Na + one e - (color center) antiferromagnetic (AFM) order of e - Energy (relative stability) color center e-e-

23
SES AFM order between color centers (e - ) G.K.H. Madsen, Bo B. Iversen, P. Blaha, K. Schwarz, Phys. Rev. B 64, 195102 (2001) Spin density -

24
INVAR alloys (invariant) e.g. Fe-Ni Such systems essentially show no thermal expansion around room temperature

25
INVAR (invariant) of Fe-Ni alloys The thermal expansion of the Eifel tower Measured with a rigid Fe-Ni INVAR wire The length of the tower correlates with the temperature Fe 65 Ni 35 alloy has vanishing thermal expansion around room temperature Ch.E.Guillaume (1897)

26
Magnetostriction and Invar behaviour What is magnetostriction? Magnetostriction s0 is the difference in volume between the volume in the magnetic ground state and the volume in a hypothetical non-magnetic state. Above the Curie temperature the magnetic contribution m vanishes. TcTc

27
Fe-Ni Invar alloys „classical“ Fe-Ni Invar Fe 65 Ni 35 alloy has vanishing thermal expansion around room temperature

28
Early explanations of INVAR A.R.Williams, V.L.Moruzzi, G.D.Gelatt Jr., J.Kübler, K.Schwarz, Aspects of transition metal magnetism, J.Appl.Phys. 53, 2019 (1982) FCC 50% Fe 100% Fe 60 70 80 volume (Bohr) 3 γ 2 FM high moment 75% Fe large volume small moment small volume γ 1 AF fcc Fe low spin m=0.5 μ B AF a = 3.57 Å high spin m=2.8 μ B FM a = 3.64 Å R.J.Weiss Proc.Roy.Phys.Soc (London) 32, 281 (1963) kT

29
Energy surfaces of Fe-Ni alloys This fcc structure from non magnetic Fe (fcc) to ferromagnetic Ni as the composition changes At the INVAR composition There is a flat energy surface as function of volume and moment 100% % Fe 75% 50% 0% Fe-Ni alloy

30
Finite temperature Energy surface at T=0 (DFT) as a function of volume and moment using fixed spin moment (FSM) calculations Finite temperature Spin and volume fluctuations Ginzburg-Landau model T 439 K T C 300 K 200 K 100 K 0 K

31
FSM calculations fixed spin moment (FSM) e.g. Fe-Ni alloy allows to explore energy surface E(V,M) as function of volume V magnetic moment M

32
Fixed spin moment (FSM) method There are systems (e.g. like fcc Fe or fcc Co), for which the magnetization shows a hysteresis, when a magnetic field is applied (at a volume V). The volume of the unit cell defines the Wigner-Seitz radius r WS The hysteresis causes numerical difficulties, since there are several solutions (in the present case 3 for a certain field H). In order to solve this problem the FSM method was invented Hysteresis

33
Fixed spin moment (FSM) method Conventional scheme constrained (FSM) method output input output poor convergence good convergence Simple case: bcc Fe difficult case: Fe 3 Ni one SCF many calculations

34
FSM Physical situation: One applies a field H and obtains M but this functions can be multivalued Computational trick (unphysical): One interchanges the dependent and independent variable this function is single valued (unique) i.e. one chooses M and calculates H afterwards

35
FSM key references A.R.Williams, V.L.Moruzzi, J.Kübler, K.Schwarz, Bull.Am.Phys.Soc. 29, 278 (1984) K.Schwarz, P.Mohn J.Phys.F 14, L129 (1984) P.H.Dederichs, S.Blügel, R.Zoller, H.Akai, Phys. Rev, Lett. 53,2512 (1984)

36
Unusual magnetic systems GMR (Giant Magneto Resistance) half-metallic systems e.g. CrO 2 important for spintronics

37
Once upon a time, … Once upon a time, in the early 1980’s … Peter Gr ü nberg N S S N ? “What happens if I bring two ferromagnets close –I mean really close– together?”

38
The electrical resistance depends on the relative magnetic alignment of the ferromagnetic layers 19% for trilayers @RT 80% for multilayers @ RT Giant magnetoresistance (GMR) Ferromagnet Metal Ferromagnet Electrical resistance: R P ) R AP GMR is much larger than the anisotropic magnetoresistance (AMR)

39
1988: … simultaneously, but independent … Albert Fert “Does the electrical resistance depend on the magnetization alignment?” Peter Gr ü nberg

40
http://www.kva.se/ Scientific background

41
CrO 2 half-metallic ferromagnet CrO 2 (rutile structure) spin-up spin-down gap metallic i mportant for spintronics

42
CrO 2 DOS The DOS features of CrO 2 are qualitatively like TiO 2 (for spin-down) RuO 2 (for spin-up) metallic gap K.Schwarz, CrO 2 predicted as a half-metallic ferromagnet, J.Phys.F:Met.Phys. 16, L211 (1986) 45678 TiVCrMnFe ZrNbMoTcRu spin all three compound crystallize in the rutile structure

43
Half-metallic ferromagnet CrO 2 (rutile structure) spin-up spin-down gap metallic

44
CrO 2 spin-down (TiO 2 ) spin-up (RuO 2 )

45
Magnetic structure of uranium dioxide UO 2 R.Laskowski G.K.H.Madsen P.Blaha K.Schwarz topics non-collinear magnetism spin-orbit coupling LDA+U (correlation of U-5f electrons) Structure relaxations electric field gradient (EFG) U O R.Laskowski, G.K.H.Madsen, P.Blaha, K.Schwarz: Magnetic structure and electric-field gradients of uranium dioxide: An ab initio study Phys.Rev.B 69, 140408-1-4 (2004)

46
Atomic configuration of uranium (Z=92) nrel j (relativ.) n ℓℓ-sℓ+s 7s-0.25 6d-0.29-0.25 5f-0.17-0.11 6p-1.46-2.10 6s-3.40 5d-7.48-6.89 5p-18.05-14.06 5s-22.57 4f-27.58-26.77... 1s-8513.38 U [Xe] 4f 14 5d 10 6s 2 6p 6 5f 3 6d 1 7s 2 core semi-core valence E j (Ryd) [Rn] core-like delocalized

47
non-collinear magnetism in UO 2 collinear 1k- non-collinear 2k- or 3k-structure

48
UO 2 2k structure, LDA+SO+U Magnetisation direction perpenticular at the two U sites (arrows) Magnetisation density (color) U O

49
Magnetism with WIEN2k

50
Spin polarized calculations

51
Run spin-polarized, FSM or AFM calculations

52
Various magnetism cases

53
Thank you for your attention

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google